Single Step Solid-Solid Reaction Scheme for the Synthesis ... · Title: Single Step Solid-Solid...
Embed Size (px)
Transcript of Single Step Solid-Solid Reaction Scheme for the Synthesis ... · Title: Single Step Solid-Solid...
Advances in Nanoparticles, 2013, 2, 28-31 http://dx.doi.org/10.4236/anp.2013.21006 Published Online February 2013 (http://www.scirp.org/journal/anp)
Single Step Solid-Solid Reaction Scheme for the Synthesis of Cobalt Sulphide-Oxide Nanoparticles in Polymer Matrix
Narendra Rumale1,2, Sudhir Arbuj2, Govind Umarji2, Manish Shinde2, Uttamrao Mulik2, Anuj Pokle3, Dinesh Amalnerkar2*
1ELANTAS Beck India Ltd., Pimpri, India 2Centre for Materials for Electronics Technology (C-MET), Panchawati, India
3Icon Analytical Equipment Pvt. Ltd., Mumbai, India Email: *[email protected]
Received December 14, 2012; revised January 15, 2013; accepted January 25, 2013
ABSTRACT At present, there is considerable interest in polymer-metal chalcogenides/oxides based nano-composites on account of their tunable optical, magnetic, electronic and catalytic properties. Here in, we report a simple single step approach for the in-situ synthesis of combined cobalt sulphide/cobalt oxide in polyphenylenesulphide (PPS) polymer matrix. We have illustrated the suitability of this methodology by reacting commonly available cobalt precursors with engineering thermoplastic, PPS. The cobalt precursor was homogeneously mixed with PPS in the molar ratios of 1:1, 1:5, 1:10, 1:15, respectively, followed by heating the mixtures obtained at the melting temperature of the polymer (285˚C) for six hours. The resultant products were characterized by X-ray Diffractometry (XRD), Field-Emission Scanning Electron Micros-copy (FESEM), High Resolution Transmission Electron Microscope (HRTEM), Diffuse Reflectance Spectroscopy (DRS) technique and Fourier Transformation Infra red Spectroscopy (FTIR). Formation of mixed phases viz., sulphide and oxide of cobalt within modified PPS matrix was confirmed by XRD. The resultant nanoparticles of cobalt sulphide and cobalt oxide embedded in the PPS matrix showed crooked and chunk morphology. The optical properties of the resultant nanocomposites indicate the shift in the absorption hump due to nanoscale size effect. Keywords: Polymers; Nanocomposites; Cobalt Sulphide/Oxide; Solid-Solid Reaction
1. Introduction In the recent times metal sulphides-oxides embedded in polymeric matrices have represented a new class of nano- structured materials. These materials combine the prop-erties of the polymer as well as the metal and its corre-sponding sulphide-oxide and show entirely a different set of properties in comparison to the original materials. These materials coalesce various properties such as opti-cal transparency, magnetism, luminescence, UV-visible absorption etc. leading to exclusive functional materials that can be easily explored for numerous applications in different technological fields . The transition metal sulfide nanomaterials have been the focus of consider-able interest due to their unique optical and electrical properties and their wide variety of potential applications in nanoscale devices such as electroluminescence and nonlinear optical devices . Cobalt sulphide-oxides are one of the most complicated systems known due to their number of phases and chemical compositions. Few phases of cobalt sulphide and oxides reported are CoS,
Co3S4, CoS2, Co9S8, CoO, Co3O4 etc. Cobalt sulphide/ oxides are one of the important classes of material which have found direct applications in solar selective coatings, photo detectors, solar cells, biological labeling, Li-ion battery, and magnetic devices etc. [3,4]. These materials have gained immense importance in recent time due to their magnetic properties and their use for fabrication of dilute magnetic semiconductor materials. Till date nu-merous techniques have been used for the synthesis of nanoscale cobalt sulphide and oxide nano-particles sepa-rately such as anodized alumina films for growth of co-balt disulphide nanowires by application of two electrical fields , colloidal synthesis of hallow nano-cobaltsul-phide spheres , hallow metal oxides and sulphides by laser ablation in liquid , hydrothermal technique , biomolecule-assisted hydrothermal process , cobalt sulfide in montmorillonite by solid-solid reaction , co-precipitation method for generation of cobalt oxide nanoparticles [11,12], chemical bath deposition of thin films , Co3O4 nanowalls by direct heating of cobalt foil on hot plate etc. . In addition to the above, num-ber of methods have been reported for in-situ generation *Corresponding author.
Copyright © 2013 SciRes. ANP
N. RUMALE ET AL. 29
of well defined nanoparticles in polymeric matrices such as ring opening metathesis polymerization (ROMP) to synthesize cobalt diblock copolymer , atom transfer radical polymerization (ARTP), nitroxide mediated po-lymerization (NMP), reverse addition fragmentation chain polymerization (RAFT) etc. .
In this communication, we report one step approach for the synthesis of cobalt sulphide-oxide nanoparticles in thermally stable polymer matrix of polyphenylenesul-phide (PPS) by simple polymer inorganic solid-solid re-action scheme. The polymer PPS has been intentionally chosen as it serves dual purpose-first it acts as a chalco-gen source and second it acts as a stabilizing media. The advantage of synthesizing semiconductor nanoparticles in the polymer matrix is that it provides good stabiliza-tion action and controls the agglomeration of nano-par-ticles formed within the polymer matrix.
2. Experimental Details The reactant cobalt nitrate was obtained from Merck and was used as received, the polymer polyphenylenesulphide (PPS) with number average molecular weight 10,000 having glass transition temperature (Tg) 88˚C with melt-ing temperature of 285˚C was obtained from Sigma Al-drich. The material was synthesized by reacting the pre-cursors in the molar ratio of 1:1, 1:5, 1:10, 1:15, respec-tively, for cobalt nitrate and PPS. The materials for each molar ratio were mixed using agate mortar and pastel and a few drops of acetone were added for proper wetting of the reactants. The admixtures thus formed were then heated at the melting temperature of the polymer i.e. 285˚C for six hours in a muffle furnace under normal atmospheric conditions. The phase identification of the resultant powder products was conducted using X-ray diffractometer (Brucker D5005), using CuK radiation. Material in powdered form was used for such analysis. The particle size and the surface morphology of the sam-ples were investigated by HRTEM with FEI Tecnai G2, at an acceleration voltage of 200 KV. The samples for HRTEM were prepared by dispersing fine powder of the resultant product in isopropyl alcohol. The dispersion was than coated on carbon coated grid for further analy-sis. The surface morphology was determined using FE-SEM, Hitachi, S-4800, the solid samples were used as such for determination. In order to prevent the charging effect associated with FESEM, the samples were placed on carbon tape and coated with thin Au film. The Infra-red study was carried out using Fourier transformation Infrared spectrophotometer (FTIR-Perkin Elmer Spec-trum 100). Approximately 500 mg of sample was mixed with dried KBr powder, the mixture was grinded and pellets were formed for further IR analysis. The UV-DRS spectra were recorded on UV 3600, Shimadzu UV-VIS- NIR spectrophotometer for solid powder samples.
3. Results and Discussion Figure 1 depicts the XRD pattern obtained for the resul-tant products. Prominent formation of Co3O4 for the 1:1 and 1:5 ratio of ratio of cobalt nitrate to PPS is observed (Figures 1(a) and (b)). The diffraction peak at 2 value of 36.8, 44.8, 59.3 and 65.2 respectively corresponds to (311), (400) planes, (511) and (440) indicating the for-mation of cubic Co3O4 (JCPDS No.42-1467). For sam-ples corresponding to 1:10 and 1:15 precursor to PPS ratio, mixed phases of Co3S4 and Co3O4 were obtained with dominance of Co3O4 phase. This substantiates that the sulphur moiety from the polymer has reacted with the cobalt precursor. The diffraction peak at 26.7, 31.4, 38.1, 55.1 correspond to cubic Co3S4, (JCPDS No. 47-1738) whereas the peak at 36.8 corresponds to Co3O4. The peak observed at 2 value of 20.5˚ in Figures 1(b)-(d) matches with PPS.
The images in Figure 2 elucidate the FESEM images for the obtained nanocomposites for the various ratios of cobalt precursor to PPS polymer. Formation of irregular shape morphology having size in the range of 30 nm to 100 nm is observed for the 1:1 ratio (Figure 2(a)). Uni-form distribution of the Co3S4 and Co3O4 is observed for the higher proportion of PPS (Figures 2(c) and (d)). The composition with 1:10 cobalt to polymer shows uniform distribution with the average particle size of 30 nm.
The HRTEM analysis is shown in Figure 3. The for-mation of nanoparticles embedded in the PPS matrix is observed for the Co3O4 prepared using 1:1 ratio. The average particle size for the resultant composition was found to be in between 5 to 10 nm. The SAED pattern shown as inset of Figure 3(a) indicates the formation of cubic Co3O4, which is also evident from the XRD analy-sis for the resultant nanocomposites. The interplanar
10 20 30 40 50 60 70 80
Figure 1. XRD patterns of Co3O4 and Co3S4, samples of Cobalt to PPS ratios where (a) 1:1, (b) 1:5, (c) 1:10, (d) 1:15 (♦) indicates oxide peaks, (●) indicates sulphide peaks and () corresponds to PPS peak. Pink line indi-cates the JCPDS No. (47-1738) corresponding to Co3S4 and green line indicates the JCPDS No. (42-1467) corre-sponding to Co3O4.
Copyright © 2013 SciRes. ANP
N. RUMALE ET AL. 30
Figure 2. FESEM images for the resultant products for different ratios of Cobalt Nitrate precursor to PPS where (a) 1:1, (b) 1:5, (c) 1:10 and (d) 1:15. (Scale bars: 300 nm for Figure (a) and 500 nm for Figures (b)-(d), respectively).
Figure 3. HRTEM images for the material for different ratios of Cobalt Nitrate precursor to PPS where (a) 1:1, (b) 1:5, (c) 1:10 and (d) 1:15.
spacing of 0.24 and 0.28 corresponds to (311) and (220) planes, respectively, thereby indicating the formation of crystalline Co3O4. HRTEM analysis of nanocomposites prepared using 1:5 ratio also indicates formation nano sized Co3O4 having size in the range of 5 to 10 nm. Slight agglomerations of nano particles are observed. The SAED pattern and the lattice spacing (Figures 3(b) and (b')) confirms the formation of cubic Co3O4 and also supports the XRD analysis. For higher ratio (1:10 and 1:15) the formation of distorted rod like morphology was observed. The SAED pattern and lattice spacing indicates the formation of Co3S4 (Figures 3(c), (c') and (d), (d')) with lattice spacing of 0.2855 matching well with (311) plane of Co3S4.
DRS spectra of prepared nanocomposites are depicted in Figure 4. PPS indicates the absorption edge at 390 nm. The band edge of the nanocomposites was located at 790 nm (1.5 eV), had a blue shift of approximately 288 nm with respect to the band gap of 1078 nm (1.15 eV) for bulk Co3S4. The hump centered at 750 nm corresponds to the band gaps of Co3O4 and Co3S4 which, interestingly, are almost in the same range [17,18].
The FTIR spectra obtained for neat PPS and the resul-tant nanocomposites are depicted in Figure 5. Character- istic bands of PPS are observed at 1471 cm−1 due to stretching vibration of C=C in benzene and 818 cm−1 due
200 300 400 500 600 700 800
PPS 1:1 1:5 1:10 1:15
Figure 4. DRS of pure PPS and samples prepared using cobalt salt to PPS ratios of 1:1, 1:5, 1:10, 1:15, respec-tively.
Figure 5. FTIR spectra of pure PPS and samples pre-pared using cobalt salt to PPS ratios of 1:1, 1:5, 1:10, 1:15, respectively.
Copyright © 2013 SciRes. ANP
N. RUMALE ET AL.
Copyright © 2013 SciRes. ANP
to deformation vibration of =C-H in 1, 4 place of ben-zene, also numerous sharp bands at 1091 cm−1, 1008 cm−1, and 485 cm−1 which may be attributed to the crys-talline nature of PPS are observed in Figure 5(a). In the spectra for nanocomposites of various ratios (Figures 5(b)-(e)), the peaks at 624 cm−1 are characteristics of metal oxide bands. A peculiar peak at 2030 cm−1 is ob-served for the resultant nanocomposites.
4. Conclusion In summary, we have successfully synthesized cobalt sulphide/oxide nanoparticles in polymer matrix by facile solid-solid reaction technique. The formation of cubic structure Co3O4 and Co3S4 embedded in the PPS matrix was confirmed by XRD and HRTEM. This technique, being quite simple, can be used for preparation of nano-composites for future generation smart materials. The polymer PPS being an engineering thermoplastic with inherent flame retardant characteristics can be molded as desired for advanced device fabrication.
5. Acknowledgements One of the authors (N. P. Rumale) sincerely acknowl-edges to the Managing Director of ELANTAS Beck In-dia Ltd. Mr. Rajeev Bhide, the Managing Director of Icon Analytical Equipment Pvt. Ltd., Mr. Anand Rao, Dr. B. B. Kale, Scientist, Centre for Materials for Electronics Technology (C-MET) for their kind support in carrying out this work.
REFERENCES  L. F. Nicolais and G. Carotenuto, “Synthesis of Poly-
mer-Embedded Metal, Semimetal, or Sulfide Clusters by Thermolysis of Mercaptide Molecules Dissolved in Poly-mers,” Recent Patents on Materials Sciences, Vol. 1, No. 1, 2008, pp. 1-11. doi:10.2174/1874464810801010001
 X. H. Liu, “Hydrothermal Synthesis and Characterization of Nickel and Cobalt Sulfides Nanocrystallines,” Materi-als Science and Engineering B, Vol. 119, No. 1, 2005, pp. 19-24. doi:10.1016/j.mseb.2004.12.051
 L. P. Deshmukh and S. T. Mane, “Liquid Phase Chemical Deposition of Cobalt Sulphide Thin Films: Growth and Properties,” Digest Journal of Nanomaterials and Bio-structures, Vol. 6, No. 3, 2011, pp. 931-936.
 H. Yang, Y. Hu, X. Zang and G. Qui, “Mechanochemical Synthesis of Cobalt Oxide Nanoparticles,” Materials Let-ters, Vol. 58, No. 3-4, 2004, pp. 387-389. doi:10.1016/S0167-577X(03)00507-X
 G. H. Yue, P. X. Yan, X. Y. Fan, M. X. Wang, D. M. Qu, Z. G. Wu, C. Li and D. Yan, “Structure and Properties of Cobalt Disulfide Nanowire Arrays Fabricated by Elec-trodeposition,” Electrochemical and Solid-State Letters, Vol. 10, No. 3, 2007, pp. D29-D31. doi:10.1149/1.2430564
 Y. Yin, C. K. Erdonmez, A. Cabot, S. Hughes and A. P. Alvistatos, “Colloidal Synthesis of Hollow Cobalt Sulfide Nanocrystals,” Advanced Functional Materials, Vol. 16, No. 11, 2006, pp. 1389-1399. doi:10.1002/adfm.200600256
 K. Y. Niu, J. Yang, S. A. Kulinich, J. Sun and X. W. Du, “Hollow Nanoparticles of Metal Oxides and Sulfides: Fast Preparation via Laser Ablation in Liquid,” Langmuir, Vol. 26, No. 22, 2010, pp. 16652-16657. doi:10.1021/la1033146
 P. Justin and G. R. Rao, “CoS Spheres for High Rate Electrochemical Capacitive Energy Storage Application,” International Journal of Hydrogen Energy, Vol. 35, No. 18, 2010, pp. 9709-9715. doi:10.1016/j.ijhydene.2010.06.036
 S. J. Bao, Y. Li, C. M. Li, Q. Bao, Q. Lu and J. Guo, “Shape Evolution and Magnetic Properties of Cobalt Sul-fide,” Crystal Growth Design, Vol. 8, No. 7, 2008, pp. 3745-3749. doi:10.1021/cg800381e
 N. Khaorapapong, A. Ontam and M. Ogawa, “Very Slow Formation of Copper Sulfide and Cobalt Sulfide Nano- particles in Montmorillonite,” Applied Clay Science, Vol. 51, No. 1, 2011, pp. 182-186. doi:10.1016/j.clay.2010.10.030
 C. R. Indulal, G. S. Kumar, A. V. Vaidyan and R. Raveen-dran, “Oxide Nanostructures: Characterisations and Opti-cal Band Gap Evaluations of Cobalt Manganese and Nickel at Different Temperatures”, Journal of Nano- and Electronic Physics, Vol. 3, No. 1, 2011, pp. 170-178.
 K. GézaSzabó and M. Zrínyi, “Liquid-Phase Synthesis of Cobalt Oxide Nanoparticles,” Journal of Nanoscience and Nanotechnology, Vol. 11, No. 5, 2011, pp. 1-9.
 F. I. Ezema, “Preparation and Optical Characterization of Chemical Bath Deposited CdCoS2 Thin Films,” Journal of Applied Sciences, Vol. 6, No. 8, 2006, pp. 1827-1832. doi:10.3923/jas.2006.1827.1832
 T. Yu, Y. Zhu, X. Xu, Z. Shen, P. Chen, C. T. Lim, J. Thiam, L. Thong and C. H. Sow, “Controlled Growth and Field Emission Properties of Cobalt Oxide Nanowalls,” Advanced Materials, Vol. 17, No. 13, 2005, pp. 1595- 1599. doi:10.1002/adma.200500322
 S. R. Ahmed and P. Kofinas, “Magnetic Properties and Morphology of Block Copolymer-Cobalt Oxide Nano-composites,” Journal of Magnetism and Magnetic Mate-rials, Vol. 288, 2005, pp. 219-223. doi:10.1016/j.jmmm.2004.09.009
 J. Pyun, “Nanocomposite Materials from Functional Poly-mers and Magnetic Colloids,” Polymer Reviews, Vol. 47, No. 2, 2007, pp. 231-263. doi:10.1080/15583720701271294
 N. Mathur, R. K. Joshi, G. V. Subbaraju and H. K. Sehgal, “Solution Grown Pb1−xCoxS Semiconductor Nanoparticle Film,” Physica E: Low-Dimensional Systems and Nanos-tructures, Vol. 23, No. 1-2, 2004, pp. 56-60.
 L. He, Z. Li and Z. Zhang, “Rapid, Low-Temperature Synthesis of Single Crystalline Co3O4 Nanorods on Sili-con Substrates on a Large Scale,” Nanotechnology, Vol. 19, No. 15, 2008, Article ID: 155606. doi:10.1088/0957-4484/19/15/155606http://dx.doi.org/10.2174/1874464810801010001http://dx.doi.org/10.1016/j.mseb.2004.12.051http://dx.doi.org/10.1016/S0167-577X(03)00507-Xhttp://dx.doi.org/10.1149/1.2430564http://dx.doi.org/10.1002/adfm.200600256http://dx.doi.org/10.1021/la1033146http://dx.doi.org/10.1016/j.ijhydene.2010.06.036http://dx.doi.org/10.1021/cg800381ehttp://dx.doi.org/10.1016/j.clay.2010.10.030http://dx.doi.org/10.3923/jas.2006.1827.1832http://dx.doi.org/10.1002/adma.200500322http://dx.doi.org/10.1016/j.jmmm.2004.09.009http://dx.doi.org/10.1080/15583720701271294http://dx.doi.org/10.1088/0957-4484/19/15/155606